thErMOplastIc rEsINs fOr flExIblE fraMEwOrk rEMOvablE partIal ...
Review aRticleSthErMOplastIc rEsINs fOr flExIblE fraMEwOrkrEMOvablE partIal DENtUrEsMeda Negrutiu, cosmin Sinescu, Mihai Romanu, Daniela Pop, Sorin lakatosrEZUMatUtilizarea terapeutic a materialelor termoplastice a crescut semnificativ n ultimul deceniu. Aceste proceduri noi, prin care un material complet polimerizat esteplastifiat prin prelucrare termoplastic (fr a aduce modificri chimice) [i apoi injectat ntr-un tipar a deschis un nou capitol n tehnologia protezelor mobile[i mobilizabile. Biocompatibilitatea excelent [i propriet]ile mecanice superioare ale acestor materiale pot fi ob]inute doar printr-o prelucrare technologiccorespunztoare. Aplica]ile actuale ale materialelor termoplastice n medicina dentar includ: cro[ete preformate, proteze par]iale mobilizabile cu baz flexibil,coroane [i proteze par]iale fixe provizorii, [ine ocluzale, stlpi implantari, dispozitive ortodontice etc. Prin dezvoltarea de noi combina]ii de elastomeri [icopolimeri este sigur c vor aprea multe aplica]ii clinice noi ale r[inilor termoplastice n medicina dentar.Cuvinte cheie: R[ini termoplastice, proteze par]iale flexibile, sisteme de injectareabstractThe therapeutic use of thermoplastic materials has increased drastically in the late decade. This new procedure, during which a fully polymerized basic materialis softened by heat (without chemical changes) and injected afterwards, has opened up a new chapter in making dentures. The excellent tissue-friendly andmechanical characteristics of these basic materials can only be made to last by an exactly executed and reproducible technology. Current dental applications ofthermoplastic materials include: preformed partial denture clasp, flexible tooth born partial denture framework, single cast partial dentures, temporary crowns andbridges, provisional crowns and bridges, occlusal appliances, implant abutments, orthodontic and sleep apnea appliances, many of which have been describedpreviously. However, with the development of new elastomers and copolymer alloys, there are certain to be many new clinical applications for thermoplasticresins in dentistry.Key Words: Thermoplastic resin, flexible framework RPD, injection systemINtrODUctION denture teeth as replacements for the missing natural teeth. The differences between them are the materials If you are missing only a few teeth scattered over used to support the denture teeth and retain the RPDeither arch (upper or lower teeth), or even if you have in the mouth.2a minimum of two teeth on both sides of the arch, The application of nylon-like materials to thethen you can most inexpensively replace the missing fabrication of dental appliances. has been seen as anteeth with a removable partial denture (RPD). There advance in dental materials. This material generallyare several types of RPD’s.1 All of them use standard replaces the metal, and the pink acrylic denture material used to build the framework for standard removable partial dentures.3 Thermoplastic materials for dental prostheses,Department of ProsthesesTechnology and Dental Materials, Faculty of Dental Valplast (Valplast Int. Corp. - USA) and FlexiplastMedicine, Victor Babes University of Medicine and Pharmacy Timisoara (Bredent - Germay), were first introduced to dentistryCorrespondence to: in the 1950s. Both materials were similar grades ofMeda Negrutiu, PhD, DMD, Department of Prostheses Technology and Polyamides (nylon plastics). Since their introduction,Dental Materials, Faculty of Dental Medicine, 2 Eftimie Murgu Square, there has been a continued interest in thermoplasticTimisoara, Tel. +40 722 700593Email: email@example.com dental materials.4,5 Rapid Injection Systems (currently known asReceived for publication: Mar. 14, 2005. Revised: Sep. 30, 2005. The Flexite Company - USA), originated in 1962, _____________________________ Meda Negrutiu et al 295
introduced the first Flexite thermoplastic which was a very little or almost no free monomer in the material.flouropolymer (a Teflon-type of plastic).6 A significant percentage of the population is allergic Valplast introduced a flexible semi-translucent to free monomer and these materials offer a new safethermoplastic resin to create flexible tissue-born treatment alternative for these individuals. In addition,partial dentures. While the material was not strong thermoplastic materials have almost no porosity, whichenough to allow for conventional tooth born rest seat, reduces biologic material build up, odors, and stainsthe flexibility added to patient comfort in wearing the and exhibit higher dimension and color stability. Allappliances.5 of these factors become important when producing Flexite also was early into the dental market with long-term provisional prostheses during implant orflexible thermoplastic acrylic hybrid resin for removable complex restorative cases, or when used for permanentappliances. Acetal was first proposed as an unbreakable removable appliances. Typically, the thermoplasticthermoplastic resin removable partial denture material resins are more flexible and stronger than theirin 1971. It was during this period that Rapid Injection traditional counterparts are. Elastomeric resins can beSystems developed the first tooth-colored clasps with added to the resin polymer formulas to create greatera thermoplastic fluoropolymer.7 flexibility, which reduces fracturing. Thermoplastic In 1986, Dental ‘D’ reintroduced tooth-colored resins can also be reinforced with glass filler or fibers toclasps using Acetal resin. The clasps were flexible, further enhance their physical properties.9 At the samedid not need periodic adjustment to keep them tight, time, these restorations can be relined and repaired, byand the tooth colored esthetics were appreciated by repressing the restoration. The thermoplastic resinsthe patients. Pressing Dental followed in the early can produce single cast or pressed restorations that1990s with an Acetal resin, (marketed in the U.S. by are strong, lightweight, flexible appliances in tissueDENTSPLY Austenal), which in addition to tooth or tooth color matched materials that never needcolored clasps, has been used for an entire partial adjusting. These restorations display excellent estheticsdenture framework as well as other appliances.8 and provide long-term comfortable use for the patient. In 1992, The Flexite Company, developed and This provides excellent alternative cosmetic restorationspatented the first pre-formed tooth-color clasps for esthetic-conscious patients. Thermoplastic resinsknown as Clasp-Eze. This product, made of a nylon are used for a broad variety of applications frommaterial, is available in pink and clear color shades and removable flexible partial dentures, preformed partialcurrently sold worldwide. denture clasps, fiber reinforced fixed partial dentures DENTSPLY recently introduced the Success temporary crowns and bridges, provisional crownsFRS, “flexible resin system” for their Success denture and bridges, obturators and speech therapy appliances,press. The FRS system utilizes a flexible tissue colored orthodontic retainers and brackets, impression tray10thermoplastic resin for flexible partial dentures. and border molding materials11, occlusal splints, sleepCurrently Cosmetic Dental Materials, has introduced apnea appliances, and implant abutments.Aesthetic PerfectionT (patent pending), a new lineof thermoplastic Acetal, Acrylic, and Polycarbonate thErMOplastIc acEtalmaterials that can be used in most thermoplasticpresses. These materials offer excellent esthetics Acetal as a homo-polymer has good short-combined with favorable physical properties and easy term mechanical properties, but as a co-polymer hasprocessing characteristics.5 better long-term stability. Acetal resin is very strong, resists wear and fracturing, and is quite flexible.aDvaNtagEs Of thErMOplastIc These characteristics make it an ideal material forMatErIals pre-formed clasps for partial dentures, single pressed unilateral partial dentures, partial denture frameworks, Thermoplastic resins and co-polymers have provisional bridges, occlusal splints, and even implantmany advantages over conventional powder or abutments. Acetal resins resist occlusal wear and areliquid resin systems. Thermoplastic resins tend to well suited for maintaining vertical dimension duringhave predictable long-term performance. They are provisional restorative therapy.5stable and resist thermal polymer unzipping. They While stronger, Acetal does not have the naturalalso exhibit high creep resistance and high fatigue translucency and vitality of thermoplastic acrylic andendurance as well as excellent wear characteristics and polycarbonate, and these materials might offer bettersolvent resistance. Thermoplastic resins typically have results for short-term temporary restorations._____________________________296 TMJ 2005, Vol. 55, No. 3
thErMOplastIc pOlycarbONatE is a versatile material with a depth of characteristics making it suitable for a broad range of applications. Polycarbonate is a polymer chain of bisphenol-A Nylon exhibits high physical strength, heat resistancecarbonate. It is a popular material and has been used and chemical resistance. It can be easily modified toin dentistry for a long time as preformed temporary increase stiffness and wear resistance. Because ofcrown shells. Similarly to Acetal resin, polycarbonate its excellent balance of strength, ductility and heatresin is also very strong, resists fracturing, and is quite resistance, nylon is an outstanding candidate forflexible. However, polycarbonate does not wear as well metal replacement applications. However, in dentistry,as Acetal during occlusal force and consequently will because of its inherent flexibility, it is used primarilynot maintain vertical dimension as long. Polycarbonate for flexible tissue born partial dentures. It does notis ideally suited for provisional crowns and bridges have enough strength to use for occlusal rest seats,but not suitable for partial denture frameworks. The and won’t maintain vertical dimension when used inmaterial has a natural translucency and finishes very well, direct occlusal forces. Thermoplastic nylon is injectedyielding excellent esthetics. Temporary and provisional at temperatures from 274 to 293 degrees Celsius andrestorations with thermoplastic polycarbonate provide has a specific gravity of 1.14. Mold shrinkage amountspatients with excellent short or mid-term function and to 0.014 in/in. The tensile strength is 11000 psi andesthetics.7,12 the flexural strength is 16000 psi. Nylon is a little more difficult to adjust and polish, but the resin can be semi-thErMOplastIc acrylIc translucent and provides excellent esthetics for flexible tissue born partial dentures.5,12-15 Acrylic is better known as polymethyl methacrylateor PMMA. This material has been used in dentistry applIcatIONs fOr thErMOplastIcfor many years in the form of temporary crowns and rEsINsthermal polymerized as baseplate material for partialand complete dentures. Thermal polymerized PMMA Applications for thermoplastics resins originallydemonstrates high porosity, high water absorption, involved flexible tooth born partial dentures. Currentlyvolumetric changes and residual monomer. These dental applications include: preformed partial dentureproperties lead to many of the problems associated clasp, flexible tooth born partial denture framework,with thermally polymerized acrylic versus the single cast partial dentures, temporary crowns andthermoplastic version.12 Thermoplastic acrylic has poor bridges, provisional crowns and bridges, occlusalimpact resistance, but has adequate tensile and flexural appliances, implant abutments, orthodontic and sleepstrength for a variety of applications. The material is apnea appliances, many of which have been describedeasy to adjust, handle and polish. It is relineable and previously. However, with the development of newrepairable at the chair-side. Thermoplastic acrylic is elastomers and copolymer alloys, there are certain toavailable in both tooth and gingival colors, and has both be many new clinical applications for thermoplastictranslucency and vitality, providing excellent esthetics. resins in dentistry.2,16,17Like most thermoplastic resins, acrylic resin is also Valplast (Valplast Int. Corp.) is nearly unbreakable,strong, resists fracturing, and is flexible.7,13 However, is colored pink like the gums, can be built quite thin, andacrylic does not wear as well as acetal during occlusal can form not only the denture base, but the clasps asforces and consequently will not maintain vertical well. Since the clasps are built to curl around the necksdimension over long periods of time. of the teeth, they are practically indistinguishable from Flexite M.P.-a thermoplastic acrylic, is a special the gums that normally surround the teeth.3 (Fig. 1)blend of polymers and has the highest impact ratingof any acrylic. You can bounce a Flexite M.P. dentureoff the floor without cracking the base. Flexite M.P.has a surface hardness of 55-65, making it popular forbruxism appliances as well as dentures.12thErMOplastIc NylON Fig.1 Nylon is a resin derived from diamine and dibasicacid monomers. From an engineering standpoint, nylon Figure 1. A lower Valplast partial denture. _____________________________ Meda Negrutiu et al 297
Even though this denture does not rest on the natural teeth like the metal framework variety, the clasps rest on the gums surrounding the natural teeth. This tissue, unlike the gums over extraction sites, is stable and does not tend to change over time which keeps these RPD’s stable and unchanging similar to the cast metal variety. The clasps can be seen (if you look hard) on the image on Fig. 2. just under the thumb and index fingers. This type of partial denture is extremely stable and retentive, and the elasticity of the flexible plastic clasps keeps them that way indefinitely.18,19 Figure 3. Flexite Plus flexible RPDs. Flexite Supreme’s base component: is a co- polyamid. This half-soft one has much wider range2ig.2 of use and dealing with this material makes denture manufacturing faster. High molecular flexite supreme is the ultimate cast thermoplastic for removable partials. The proportional limits (memory) is comparable to precious wire and yet it is flexible. Many dentists have switched from metal to Flexite Supreme because Flexite offers the patient superior comfort, esthetics and there is no metallic taste (Fig. 4). Flexite Supreme is easy to polish and adjust in house. It can be added to Figure 2. The flexible framework RPDs - Valplast: a) initial clinical status, or relined in office or laboratory, with acrylic, when a b) the flexible RPD; c) the RPD in situ. bonding agent is applied to a non-flexing area! Cyano The Flexite Company has six different monomer Acrylate is the coupling agent that chemically bonds free plastics for fabricating RPD’s, dentures, TMJ’s, acrylic to Flexite Supreme 20. bruxism, anti-snoring devices, sports mouth guards, tooth colored clasps, Flexite-metal combination cases etc. Flexite plastics are safe, non-toxic, comfortable, biologically inert, and meets the leaching requirements for colorants. Flexite plastics are esthetically superior to other plastics. Flexite plastics are CE certified. The Fig.4 Flexite Quality Assurance Program is designed to meet the ISO 9000 rules. 20,21 Flexite Plus “flexible” partial dentures eliminate the use of metal, providing the patients with a partial denture alternative that delivers a precise fit, tissue- colored esthetics and maximum patient comfort. Flexite Plus, comparable to Flexiplast14 and Valplast, is fabricated from a flexible thermoplastic material that is Fig.4 available in three tissue shades. The base component is nylon-polyamid. This kind is extremely elastic, almost unbreakable. The use of this material takes longer than Figure 4. Flexite Supreme flexible RPDs. the other ones.5,22 The material is monomer-free, virtually Flexite MP contains fully polimerized acrylate, its unbreakable, lightweight and impervious to oral base component is methyl-metacrylate. This material fluids. Flexite Plus may also be combined with a metal was developed for making full dentures, it doesn’t framework to eliminate the display of metal labial behave elastic, but being a bit elastic, it is practically clasps.20 (Fig. 3) unbreakable. It can be polished easily.20 _____________________________ 298 TMJ 2005, Vol. 55, No. 3
Northerm’s base component: styrene acrylonitrate 3. Negruţiu M, Sinescu C, Sandu Liliana, et al. Guidelines of removable partial dentures, Ed. Marineasa, Timişoara, 2004.copolymer. Containing no acrylate, this material is for 4. Lowe LG. Flexible denture flanges for patients exhibiting undercutallergic patients. It can be combined with metals. tuberosities and reduced width of the buccal vestibule: a clinical The flexible framework RPD can replace any report. J Prosthet Dent 2004; 92(2):128-31.number of teeth in a dental arch, similar to the flipper 5. Phoenix RD, Mansueto MA, Ackerman NA, et al. Evaluation of mechanical and thermal properties of commonly used denture baseand cast metal RPD. There is, however, one type of resins. J Prosthodont 2004;13(1):17-27.removable tooth replacement device that can (legally) 6. Beaumont AJ Jr. An overview of esthetics with removable partialbe built only out of the flexible framework variety of dentures. Quintessence Int 2002;33(10):747-55.material. This is the single tooth RPD that we refer to 7. Donovan TE, Cho GC. Esthetic considerations with removable partial dentures. J Calif Dent Assoc 2003;31(7):551-7.as a NESBIT.3 (Fig. 5) 8. Negruţiu M, Bratu D, Romînu M, et al. Polimeri utilizaţi în tehnologia protezelor mobile şi mobilizabile. Revista Natională de Stomatologie 2001; IV(1):30-41. 9. John J, Gangadhar SA, Shah I. Flexural strength of heat-polymerized polymethyl methacrylate denture resin reinforced with glass, aramid or nylon fibers. J Prosthet Dent 2001;86(4):424-7. 10. Fujisawa M, Adachi K, Tsuruta S, et al. A procedure for fitting a fixed partial denture to an existing removable partial denture. J Prosthet Dent 2004;91(4):392-4. 11. Heath JR, Boru TK, Grant AA. The stability of temporary prostheticFigure 5. The single tooth RPD - NESBIT. base materials. J Oral Rehabil 1993;20(4):363-72. 12. Janda R. Prothesenkunststoffe aus werkstoffkundlicher Sicht. Quintessenz Zahntech 1997;23(5):665-72.cONclUsION 13. Negruţiu M, Romînu M, Floriţa Z, et al. Influenţa tehnologiei de prelucrare asupra calităţii polimerilor pentru proteze mobile şi Thermoplastic resins have been used in dentistry mobilizabile. Revista de Stomatologie 2001;V(1/2):107-12.for over 50 years. During that time the applications have 14. Parvizi A, Lindquist T, Schneider R, et al. Comparison of the dimensional accuracy of injection-molded denture base materials to that ofcontinued to grow, and the interest in these materials of conventional pressure-pack acrylic resin. J Prosthodont 2004;13(2):83-9.both the profession and the public has increased. The 15. Keenan PL, Radford DR, Clark RK. Dimensional change in completematerials have superior properties and characteristics dentures fabricated by injection molding and microwave processing.and provide excellent esthetic and biocompatible J Prosthet Dent 2003;89(1):37-44.treatment options. With the development of new 16. Hohmann A., Hielscher W. Lehrbuch der Zahntechnik, Band 1– Grundlagen, partielle Prothesen, Kronen– und Brückentechnik,properties, elastomers and copolymer alloys, there Fünfte Auflage, Quintessenz Verlags–GmbH, Berlin, 1999.are certain to be additional new applications for 17. Hohmann A., Hielscher W. Lehrbuch der Zahntechnik, vol.II, ed.4,thermoplastic resins in the future, to help patients with Quintessenz-Verlags GmbH, Berlin, 2001damaged or missing teeth. 18. Pardo-Mindan S, Ruiz-Villandiego JC. A flexible lingual clasp as an esthetic alternative: a clinical report. J Prosthet Dent 1993;69:245-46. 19. Hiromori K, Fugii K, Inoue K. Viscoelastic properties of denture baserEfErENcEs resins obtained by underwater test. J Oral Rehabil 2000;27(6):522-31. 21. Mirada X. Le Flexite, une alternative au matériau résine. Proth.Dent1. Caesar HH, Lehmann KM. Die Teilprothese – Grundlagen, Konstruktion 1999;20:153-4. und zahntechnische Ausführung, 3. überarbeitete Auflage, Verlag 20. Lai YL, Lui HF, Lee SY. In vitro color stability, stain resistance, and Neuer Merkur GmbH, München, 2002. water sorption of four removable gingival flange materials. J Prosthet2. Wostmann B, Budtz-Jorgensen E, Jepson N, et al. Indications for Dent 2003;90(3):293-300. removable partial dentures: a literature review. Int J Prosthodont 22. Axinn S, O’Connor RP Jr, Kopp EN. Immediate removable partial 2005;18(2):139-45. denture frameworks. J Am Dent Assoc 1977;95:583-5. _____________________________ Meda Negrutiu et al 299